A word about my personal philosophy. It is anchored in optimism. It must be, for optimisim brings with it hope, a future with a purpose, and therefore, a will to fight for a better world. Without this optimism, there is no reason to carry on. If we think of the struggle as a climb

up a mountain, then we must visualize a mountain with no top. We see a top, but when we finall yreach it, the overcast rises and we find ourselves merely on a bluff. The mountain continues on up. Now we see the ”real” top ahead of us, and strive for it, only to find we’ve reached another bluff, the top still above us. And so it goes on, interminably. Knowing that the mountain has no top, that it is a perpetual

quest from plateau to plateau, the question arises, ”Why the struggle, the conflict, the heartbreak, the danger, the sacrifice. Why the constant climb?” Our answer is the same as that which a real mountain climber gives when he is asked why he does what he does. ”Because

it’s there.” S. Alinsky

### Charge carrier transport in Cu(In,Ga)Se

2### thin-film

### solar-cells studied by electron beam induced current

### and temperature and illumination dependent current

### voltage analyses

### vorgelegt von

### Melanie Nichterwitz

### aus Konstanz

### von der Fakult¨

### at IV - Elektrotechnik und Informatik

### der Technischen Universit¨

### at Berlin

### zur Erlangung des akademischen Grades

### Doktorin der Naturwissenschaften

### Dr. rer. nat.

### genehmigte Dissertation

### Promotionsausschuss:

### Vorsitzender: Prof. Dr. G. Tr¨

### ankle

### Gutachter: Prof. Dr. H.-W. Schock

### Gutachter: Prof. Dr. B. Rech

### Gutachter: Prof. Dr. U. Rau

### Tag der wissenschaftlichen Aussprache: 10.01.2012

### Berlin 2012

### D83

### Abstract

This work contributes to the understanding of generation dependent charge-carrier trans-port properties in Cu(In,Ga)Se2 (CIGSe)/ CdS/ ZnO solar cells and a consistent model

for the electronic band diagram of the heterojunction region of the device is developed. Cross section electron-beam induced current (EBIC) and temperature and illumination dependent current voltage (IV) measurements are performed on CIGSe solar cells with varying absorber layer compositions and CdS thickness.

For a better understanding of possibilities and limitations of EBIC measurements applied on CIGSe solar cells, detailed numerical simulations of cross section EBIC profiles for varying electron beam and solar cell parameters are performed and compared to profiles obtained from an analytical description. Especially the effects of high injection conditions are considered.

Even though the collection function of the solar cell is not independent of the generation function of the electron beam, the local electron diffusion length in CIGSe can still be extracted. Grain specific values ranging from (480 ± 70) nm to (2.3 ± 0.2) µm are de-termined for a CuInSe2 absorber layer and a value of (2.8 ± 0.3) µm for CIGSe with a

Ga-content of 0.3.

There are several models discussed in literature to explain generation dependent charge carrier transport, all assuming a high acceptor density either located in the CIGSe layer close to the CIGSe/CdS interface (p+ layer), within the CdS layer or at the CdS/ZnO interface. In all models, a change in charge carrier collection properties is caused by a generation dependent occupation probability of the acceptor type defect state and the resulting potential distribution throughout the device.

Numerical simulations of EBIC and IV data are performed with parameters according to
these models. The model that explains the experimental data best is that of a p+ layer at
the CIGSe/CdS interface and acceptor type defect states at the CdS/ZnO interface. The
p+ layer leads to generation dependent transport in EBIC at room temperature, while
defect states at the CdS/ZnO interface cause a significant reduction of the photocurrent
in the red light illuminated IV characteristics at low temperatures. Electron beam
irradi-ation of the heterojunction region alters EBIC profiles temporarily, and there is enhanced
relaxation of this effect in air. In addition, the occurrence of generation dependent
charge-carrier transport is found to correlate with the presence of an ordered defect compound
(ODC) in the absorber layer. Thus, the p+ layer occurs in connection with an ordered
defect compound (ODC) layer with a lowered valence band maximum as compared to
that of the CIGSe layer and a high net p-type doping density (1017 _{cm}−3_{), possibly due}

to the passivation of donor type defect states by oxygen incorporation.

Furthermore, shallow donor type defect states at the p+ layer/CdS interface of some grains of the absorber layer possibly caused by Cd on Cu site defects explain the fact that charge-carrier transport is grain specific, i.e. inhomogeneous, in EBIC experiments.

### Zusammenfassung

Die vorliegende Arbeit leistet einen Beitrag zu einem besseren Verst¨andnis generations-abh¨angigen Ladungstransports in Cu(In,Ga)Se2(CIGSe)/ CdS/ ZnO D¨unnschichtsolarzellen.

Ein konsistentes Modell f¨ur das elektronische Banddiagramm im Bereich der Hetero¨uberg¨ange wird entwickelt. Hierf¨ur werden Messungen elektronenstrahlinduzierter Str¨ome in der Querschnittsanordnung und temperatur- und beleuchtungsabh¨angige IV Messungen an Solarzellen mit Absorberschichten mit unterschiedlicher Zusammensetzung und einer vari-ierenden CdS Pufferschichtdicke durchgef¨uhrt.

F¨ur ein besseres Verst¨andnis der M¨oglichkeiten und Grenzen von EBIC Messungen an CIGSe Solarzellen werden detaillierte numerische Simulationen von EBIC Profilen unter der Annahme variierender Elektronenstrahl- und Solarzellenparameter durchgef¨uhrt. Diese werden mit Profilen, die aus einer analytischen Beschreibung hervorgehen, verglichen. Im Speziellen werden Hochinjektionseffekte untersucht.

Obwohl die Sammlungsfunktion der Solarzelle nicht unabh¨angig von der Generations-funktion des Elektronenstrahls ist, ist eine Extraktion der lokalen Diffusionsl¨ange der Elektronen in CIGSe m¨oglich. Diese ist kornspezifisch und wird zu Werten von (480 ± 70) nm bis (2.3 ± 0.2) µm in CuInSe2 und zu (2.8 ± 0.3) µm in einer CIGSe Schicht mit

einem Ga-Gehalt von 0.3 bestimmt.

In der Literatur werden verschiedene Modelle zur Erkl¨arung der generationsabh¨angigen Ladungstr¨agersammlung diskutiert, die alle auf der Annahme einer hohen Dichte an akzeptorartigen Defektzust¨anden entweder in der CIGSe Schicht im Bereich der CIGSe/CdS Grenzfl¨ache (p+ Schicht), in der CdS Schicht oder an der CdS/ZnO Grenzfl¨ache basieren. In allen Modellen ver¨andert sich die Ladungstr¨agersammlung in Abh¨angigkeit von der gen-erationsabh¨angigen Besetzung der Defektzust¨ande und dem resultierenden Potentialver-lauf in der Solarzelle.

Im Rahmen der vorliegenden Arbeit werden numerische Simulationen unter der An-nahme von Parametern durchgef¨uhrt, die den in der Literatur diskutierten Modellen entsprechen. Die beste ¨Ubereinstimmung mit den experimentellen Daten wird erreicht wird f¨ur ein Modell einer p+ Schicht an der CIGSe/CdS Grenzfl¨ache und Akzeptoren-zust¨ande an der CdS/ZnO Grenzfl¨ache. Die p+ Schicht verursacht die generations-abh¨angigen Transporteigenschaften in EBIC bei Raumtemperatur, wohingegen die De-fektzust¨ande an der CdS/ZnO eine Verringerung des Photostroms der Solarzelle im Fall von Rotlichtbeleuchtung bei tiefen Temperaturen bedingen. Elektronenbestrahlung der Heterogrenzfl¨achenregion ver¨andert EBIC Profile tempor¨ar, und Relaxation dieses Ef-fekts findet verst¨arkt in Anwesenheit von Sauerstoff statt. Das Auftreten generations-abh¨angiger Ladungstr¨agersammlung korreliert mit der Anwesenheit einer geordneten De-fektverbindung (ordered defect compound, ODC) in der Absorberschicht. Die p+ Schicht kommt also in Verbindung mit einer ODC Phase vor, welche ein abgesenktes Valenzband im Verh¨altnis zu der CIGSe Schicht und eine hohe netto p-Dotierung aufweist, die durch die Passivierung donatorartiger Defektzust¨ande im grenzfl¨achennahen Bereich der Ab-sorberschicht durch den Einbau von Sauerstoff zustande kommen k¨onnte.

Des Weiteren erkl¨art ein flacher Donator an der p+ Schicht/CdS Grenzfl¨ache einiger K¨orner der Absorberschicht, welcher m¨oglicherweise durch CdCu Defekte verursacht wird,

die Beobachtung, dass Ladungstr¨agertransport in EBIC kornspezifisch und damit inho-mogen ist.

## Contents

1. Introduction 1

2. Theory of charge carrier transport in heterojunction solar cells 3

2.1. The pn-junction . . . 3

2.1.1. Homojunction . . . 3

2.1.2. Heterojunction . . . 6

2.1.3. Influence of interface defects . . . 7

2.2. Charge carrier collection . . . 7

2.3. IV characteristics . . . 10

2.4. Recombination . . . 12

2.5. Thermionic emission across a potential barrier . . . 16

2.6. Tunneling through a potential barrier . . . 17

3. Charge carrier transport in Cu(In,Ga)Se2 solar cells 19 3.1. Basics of Cu(In,Ga)Se2 thin-film solar-cells . . . 19

3.1.1. Solar cell configuration . . . 19

3.1.2. Material properties of Cu(In,Ga)Se2 . . . 20

3.1.3. Electronic band diagram of the solar cell . . . 22

3.2. Interfaces in Cu(In,Ga)Se2 thin-film solar-cells . . . 22

3.3. Generation dependent charge-carrier transport properties . . . 26

3.3.1. Experimental observations . . . 26

3.3.2. p+ layer at the Cu(In,Ga)Se2/CdS interface . . . 27

3.3.3. Conduction band spike and deep acceptor states in the CdS layer . 31 3.3.4. Acceptor states at the CdS/ZnO interface . . . 32

4. Generation dependent charge-carrier transport in current voltage analysis 35 4.1. Experimental method and details . . . 35

4.2. Experimental results: Red light illumination . . . 35

4.3. Modeling: ”Red kink” effect . . . 36

4.3.1. p+ layer at the CuInSe2/CdS interface . . . 37

4.3.2. Conduction band spike and deep acceptor states in the CdS layer . 39 4.3.3. Acceptor states at the CdS/ZnO interface . . . 40

4.4. Conclusions . . . 42

5. Charge carrier transport studied by electron-beam induced current 43 5.1. Experimental method and details . . . 43

5.1.1. Measuring principle . . . 43

ii Contents

5.1.2. Electron beam generation . . . 44

5.1.3. Extraction of the minority charge-carrier diffusion length . . . 46

5.1.4. Experimental setup and details . . . 48

5.2. Modeling: Cross section electron-beam induced current . . . 49

5.2.1. Low injection: Comparison to analytical model . . . 50

5.2.2. High injection effects in electron beam induced current . . . 53

5.2.3. Conclusions . . . 57

6. Investigation of charge carrier transport in Cu(In,Ga)Se2 solar cells 59 6.1. CuInSe2 solar cells . . . 59

6.1.1. Generation dependent charge-carrier transport properties . . . 59

6.1.2. Electron-beam irradiation induced changes of transport properties . 61 6.1.3. Grain specific charge-carrier transport properties . . . 62

6.1.4. Solar cell without generation dependent charge-carrier transport properties . . . 66

6.1.5. Extraction of electron diffusion length I . . . 66

6.1.6. Summary and conclusions . . . 68

6.2. Modeling of generation dependent charge-carrier transport properties . . . 68

6.2.1. p+ layer at the CISe/CdS interface . . . 69

6.2.2. p+ layer and interface donor at the CISe/CdS interface . . . 75

6.2.3. Acceptor states in the CdS layer . . . 82

6.2.4. Acceptor states at the CdS/ZnO interface . . . 88

6.2.5. Extraction of electron diffusion length II . . . 91

6.2.6. Conclusions . . . 92

6.3. Cu(In,Ga)Se2 solar cells . . . 95

6.3.1. Variation of the Ga-content of the CIGSe absorber layer . . . 95

6.3.2. CdS thickness variation . . . 100

6.3.3. Variation of the Cu-content of the CIGSe absorber layer . . . 104

7. Implications for solar cell performance 109

8. Summary and conclusions 115

A. Simulation parameters 119

B. Solar cell parameters and absorber layer compositions 123

Bibliography 129

## 1. Introduction

Thin-film solar-cells with polycrystalline Cu(In,Ga)Se2 (CIGSe) absorber layers provide

a good alternative to wafer based crystalline silicon solar cells, which currently constitute the major share of photovoltaics installed and used worldwide. In contrast to silicon, CIGSe is a direct semiconductor material meaning that a layer thickness of some micro-meters is sufficient for absorption of most of the incoming sunlight without the necessity of light trapping structures, which have to be used in silicon thin-film devices.

CIGSe based solar cells consist of a multilayer stack of semiconductor and metallic layers. Due to the complexity of the structure with two heterojunctions involved, charge carrier transport is still not understood completely in these devices. There are several open ques-tions with respect to charge and defect distribuques-tions, band alignment and the influences on charge carrier transport. The main aim of this work is to gain a better understanding in this regard, to develop a consistent model for the electronic band diagram with a focus on the heterojunction region in equilibrium and under illumination, and to draw conclu-sions about the limiting factors for the solar conversion efficiency.

One important finding reported in literature is the occurrence of generation dependent charge-carrier transport properties observed in electron beam induced current (EBIC) measurements on cross sections of CIGSe solar cells [1] and temperature dependent cur-rent voltage (IV) analysis [2–4]. The understanding of these effects might one of the keys to a better understanding of charge-carrier transport properties within the solar cell un-der illumination. There are several explanatory models, all based on the assumption of a high density of acceptor type defect states either located at the surface of the CIGSe layer (p+ layer) [4, 5], within the CdS layer [2, 3, 6] or at the CdS/ZnO interface [7, 8]. All models have in common that for generation conditions leading to a low hole density in the heterojunction region of the solar cell, the acceptor states are mostly occupied with electrons and the high local negative charge density leads to a drastic decrease of the collected current.

For the present work, cross section EBIC and IV measurements were performed on a vari-ety of CIGSe/CdS/ZnO solar cells with varying properties with respect to their absorber composition and CdS buffer layer thickness. The advantage of the applied combination of techniques is to obtain both, spatially resolved and integral information about charge carrier transport for different generation conditions in the solar cell. One dimensional numerical simulations were carried out to reproduce the experimental data, exclude or confirm the existing explanatory models and draw conclusions about a consistent model for space charge distributions and interface properties and the resultant charge-carrier transport properties.

The outline of this thesis is as follows:

2 Chapter 1. Introduction

• In Chapter 2, the theoretical framework of charge carrier transport within a hetero-juction solar cell is provided and basic equations are given.

• In Chapter 3, the fundamentals of CIGSe solar cells and a literature survey of relevant aspects concerning charge carrier transport in CIGSe solar cells are given. In Section 3.1, the stacking sequence of the solar cell, the deposition processes, material properties of CIGSe and the electronic band diagram of CIGSe solar cells are introduced. Interface properties and their influence on charge carrier transport are treated in Section 3.2. Section 3.3 summarizes the experimental findings and explanatory models for the experimentally observed generation dependent current decrease.

• In Chapter 4, experimental results and numerical simulations concerning the so called ”red kink” effect occurring in IV measurements performed at low tempera-tures using only the red part of the light spectrum are presented. The aim is to identify and quantify the relevant parameters for a consistent explanation of the experimental data.

• In Chapter 5, EBIC is introduced as an experimental technique. In Section 5.1, the fundamentals of cross section EBIC measurements are given and an analytical model for the description of experimental data is introduced. In Section 5.2, the validity of the analytical description is tested by a comparison to numerical simulations and the influence of electron beam and solar cell parameters on EBIC data is discussed in detail. These simulations and considerations help to establish a more profound understanding of the experimental technique and its possibilities and limitations. • In Chapter 6, the results of EBIC and IV measurements on CIGSe solar cells and

nu-merical simulations are presented and used in order to develop a consistent model for the electronic band diagram of the heterojunction region of the solar cell and charge carrier transport. In Section 6.1, the experimental results of cross section EBIC measurements on a CuInSe2 (CISe) solar cell are presented. Section 6.2 summarizes

numerical simulations of EBIC and IV data performed in order to identify the origin of the experimentally observed generation dependent current decrease. In Section 6.3, EBIC and IV results obtained from series of CIGSe solar cells with different CdS buffer layer thicknesses and absorber layers of different Ga- and Cu-content are presented.

• In Chapter 7, implications of the suggested model for solar cell performance at room temperature under white light illumination, i.e. standard working conditions of the solar cell, are discussed in detail.

• In Chapter 8, the results of the present work are summarized and final conclusions are drawn.

## 2. Theory of charge carrier transport in

## heterojunction solar cells

### 2.1. The pn-junction

In this section, a brief introduction into the fundamentals of pn-junctions is given. First, the formation and basic equations of homojunctions, i.e. pn-junctions between a p-doped and an n-doped region of the same semiconductor material, is treated in Section 2.1.1. The pn-junction in standard CIGSe solar cells consisting of a layer stack of three different materials of different permittivities, doping types and densities, bandgap energies and electron affinities (CIGSe/CdS/ZnO) is a heterojunction. The theory of heterojunctions according to the Anderson model [9] will be introduced in Section 2.1.2.

### 2.1.1. Homojunction

A pn-junction forms if a p-type and an n-type semiconductor are in contact. In ther-modynamical equilibrium, the electrochemical potential is the same on the p- and the n-side. In a simple picture, the diffusion current of electrons from the n- to the p-side and of holes vice versa induced by the difference in chemical potential of p- and n-side is counterbalanced by a drift current of electrons and holes in the opposite direction, which is induced by the difference in electrical potentials of p- and n-side resulting from the spatial separation of charged particles. A space charge region with charged ionized atoms develops between the two layers, which is depleted of mobile charge carriers. The potential drop across the space charge region, which is called built in voltage Vbi, is given

by [10]:

eVbi = e(ϕ(−∞) − ϕ(∞)) = Eg− ¯EFp− ¯EFn, (2.1)

where ϕ is the electrical potential, ¯EFp is the absolute value of the energetic difference

between Fermi level and valence band maximum in the neutral region of the p-side and ¯

Efn is the absolute value of the energetic difference between Fermi level and conduction

band minimum in the neutral region of the n-side.

Within the Boltzmann approximation, which is valid if the electron and hole densities n and p are not too high, i.e. for exp|EC,V−EF|

kT

1, where EC denotes the conduction

band minimum, EV the valence band maximum and EF the Fermi energy, the charge

carrier densities are given by n = NCexp

−E¯Fn kT and p = NVexp −E¯Fp kT . Using the 3

4 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

Boltzmann approximation and using np = NCNVexp

−Eg

kT

= n2

i, the following equation

is obtained [10]:
eVbi = kT ln
N_{d}Na
n2
i
, (2.2)

if assuming that all doping atoms are ionized n = Ndand p = Na. Nastands for the doping

density of the p-type semiconductor, Ndis the doping density of the n-type semiconductor,

niis the intrinsic charge carrier density of the material and e is the elemental charge. The

spatial dependence of the electrical potential ϕ(~x) can be obtained by integration of the Poisson equation:

−∆ϕ(~x) = ρ(~x) 0

, (2.3)

where 0 denotes the electric constant, the relative permittivity of the semiconductor

material and ρ(~x) the local charge density. If assuming translation invariance parallel to the pn-junction, the problem can be restricted to one dimensional equations.

The frequently used Schottky approximation of a pn-junction assumes abrupt changes in charge density at the edges of the space charge region and at the interface between the p- and the n-side of the pn-junction. In Figure 2.1, the spatial dependence of the potential, the charge density across a pn-junction within the Schottky approximation and the electronic band diagram of this homojunction are shown.

(a) (b)
ρ
*eN*a
*-eN*d
0
φ
*-x*n 0 *x*p
*V*bi
+
-+
+
+ + +
*-E*
Position*x*

**χ**

*E*g

*w*SCR

*x*p

*-x*n n-type p-type + -+

*--eφ*

*E*C

*E*V

*E*F

Figure 2.1: (a) Space charge density ρ and electrical potential ϕ of a pn-junction within the Schottky approximation (b) Electronic band diagram of a homojunction.

xp and −xn stand for the positions of the edge of the space charge region, Eg

for the bandgap energy and χ for the electron affinity. EC and EV stand for the

conduction band minimum and the valence band maximum, wSCR for the total

width of the space charge region and EF for the Fermi level.

2.1 The pn-junction 5

where xp denotes the width of the space charge region on the p-side of the junction and

xn that on the n-side, the following equation is obtained for the ratio of the widths of the

space charge region:

xp=

Nd

Na

xn (2.4)

Thus, if Nd Na, the width of the space charge region on the p-side is much larger than

that on the n-side. The total width of the space charge region wSCR is given by:

wSCR = xp+ xn= 1 + Nd Na xn (2.5)

Integration of the Poisson equation on the n-side of the junction assuming as boundary conditions E(−xn) = 0 and ϕ(−xn) = ϕ(−∞) yields:

ϕn(x) =

eNd

20

(x + xn)2+ ϕ(−∞) (2.6)

and correspondingly on the p-side, it is obtained that:

ϕp(x) =

eNa

20

(x − xp)2+ ϕ(∞) (2.7)

assuming as boundary conditions E(xp) = 0 and ϕ(xp) = ϕ(∞). Using that ϕn(0) =

ϕp(0), the following equation for the built in potential is derived:

Vbi= ϕ(−∞) − ϕ(∞) =

e 20

(NDx2n+ Nax2p) (2.8)

By use of Equations 2.4 and 2.5, it is obtained that:

xn =
20
e
Na
Nd(Na + Nd)
Vbi
1_{2}
xp =
20
e
Nd
Na(Na+ Nd)
Vbi
1_{2}
wSCR =
20
e
Na+ Nd
NaNd
Vbi
1_{2}
(2.9)

If ϕ(−∞) =: 0, Equation 2.7 can be used to calculate the voltage drop in the p-type layer by inserting Equations 2.4 and 2.8:

ϕ(x = 0) = eNa
20
x2_{p} = Vbi
Nd
Na+ Nd
(2.10)
Thus, if Nd Na, most of the voltage drops across the p-type layer.

6 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

### 2.1.2. Heterojunction

In heterojunction devices like e.g. in CIGSe solar cells, the valence and/or the conduction band are not continuous at the interface between the different materials, they exhibit offsets. Within the Anderson model [9], charged interface states and dipoles are neglected. In the following, a heterojunction between a p-type absorber layer and an n-type window layer is considered. The bandgap energy of the window layer is assumed to be larger than that of the absorber layer: Eg,win > Eg,abs. The band offsets in valence and conduction

band ∆EV and ∆EC at the interface between the materials are given by [11]:

∆Eg = ∆EC+ ∆EV

∆EC = (χwin− χabs)e

∆EV = (χwin− χabs)e + Eg,win− Eg,abs, (2.11)

where χwin and χabs denote the electron affinities of the window and the absorber layer

materials. The built in voltage is given by:

−eVbi= Eg,abs− ¯EFp− ¯EFn+ ∆EC. (2.12)

In Figure 2.2 (b), the electronic band diagram of a window/absorber heterojunction is shown. In this case, the electron affinity of the n-type window layer is smaller than that of the p-type absorber layer resulting in a positive conduction band offset at the interface (denoted as spike).

### (a)

### (b)

Figure 2.2: (a) The n-type window layer and the p-type absorber layer are not in contact. (b) Electronic band diagram of a pn-heterojunction.

2.2 Charge carrier collection 7

### 2.1.3. Influence of interface defects

So far, the influence of additional deep defects and charged interface defects has been neglected. Especially the latter might play a crucial role concerning charge and potential distributions within CIGSe solar cells. The occupation probability f of an energetically discrete interface defect state in equilibrium is given by the Fermi distribution function:

f (Et) =

1 exp Et−EF

kT + 1

, (2.13)

where EF denotes the Fermi energy and Et the energy level of the defect state. Thus, the

charge qIF accumulated in an interface defect of density NIF with an energy level at EIF

above the valence band maximum is given by:

qIF,d = NIF,d
1 − 1
exp
_{E}
IF,d−EF
kT
+ 1
qIF,a = −NIF,a
1
exp
_{E}
IF,a−EF
kT
+ 1
(2.14)

where the subscripts a and d are used for acceptor and donor type defects, i.e. negative and positive interface charge. Thus, the charge neutrality condition for an absorber/window solar cell with charged interface defects reads:

eNd,winxn− eNa,absxp+ qIF= 0 (2.15)

Depending on their density and energetic position and in consequence occupation proba-bility, interface defects can change charge and potential distributions within the solar cell completely and can thus play a major role in charge-carrier transport processes.

By altering the field and potential distribution throughout the solar cell device, a change in local charge distributions can have a severe impact on charge-carrier transport processes. In this way, the equations and considerations of the previous section provide the basis for an understanding of the generation dependent transport properties, which are treated in detail in the present work.

### 2.2. Charge carrier collection

Charge carrier collection across the pn-junction

A solar cell is a structure which transforms the energy contained in the incident photon current of light into an external electrical current or voltage, i.e. into electrical energy. For

8 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

standard pn-junction solar cells, photons of sufficient energy are absorbed and electron-hole pairs are generated within the semiconductor layer(s). These charge carrier pairs can either recombine or they are ”collected”, which means that they get seperated and are in consequence measurable as an external current or a voltage.

For this process, ”selective” contacts for each type of charge carrier are needed. Upon irradiation, a gradient of the electrochemical potential of electrons and holes (of the electron and hole (quasi) Fermi level) develops, which causes an electron current to one contact and a hole current to the second one. In many pn-junction solar cell, this is provided by the potential drop of the space charge region (SCR) of the pn-junction and ohmic (or low barrier) contacts to the external circuit. In CIGSe thin-film solar cells, most of the electron-hole pairs are generated in the p-type CIGSe absorber layer and electrons move in direction of the pn-junction and holes to the back contact. For low injection conditions, i.e. if the density of generated charge carriers is much lower than the CIGSe doping density, the collected current is limited by the minority charge carrier (i.e. electron) current, which in turn is limited by recombination processes either in the bulk of the absorber layer, in its space charge region or at the heterointerfaces. The electron and hole current densities ~je and ~jh can be expressed as a sum of a diffusion and a drift

term [12]:

~je = ~jdiffusion,e+ ~jdrift,e= −eDe∇n + σeE~

~jh = ~jdiffusion,h+ ~jdrift,h= −eDh∇p + σhE~ (2.16)

where De,h denotes the diffusion coefficient of electrons/holes, σe,h the respective

conduc-tivity, n the electron concentration and p the hole densities and ~E an electrical field.

Charge carrier collection in the quasi neutral region

The basic equation for charge carrier transport is the continuity equation ∂ρ_{∂t} + ∇~j = 0,
which can be transformed into the following equations for the electron and hole
concen-trations n(~x) and p(~x) by use of Equation 2.16:

Dh∆p(~x) − µhE(~~ x)∇p(~x) − µhp(~x)∇ ~E(~x) − R(~x) + g(~x) = 0

De∆n(~x) + µeE(~~ x)∇n(~x) + µen(~x)∇ ~E(~x) − R(~x) + g(~x) = 0, (2.17)

where µe,h denotes the electron/hole mobility, R(~x) is the recombination rate and g(~x) is

the rate with which charge carriers are generated.

In the following, the quasi neutral region of a p-type material under low injection condi-tions is considered ( ~E = ~0). ΣBCdenotes the plane of the back contact and Σp that of the

edge of the space charge region. For point like generation at position ´~x, the density of ex-cess electrons δn(~x) obeys the following differential equation derived from the continuity equation [13]:

De∆δn(~x) −

δn(~x)

τ = a

2.2 Charge carrier collection 9

where τ is the electron lifetime and a∗ = 1s−1. The recombination rate R(~x) is approxi-mated by δn(~x)/τ in this equation. The appropriate boundary conditions are:

δn(~x) = 0 if ~x ∈ Σp

De∇δn(~x) ˆeBC = SBCδn(~x) if ~x ∈ ΣBC.

SBC corresponds to the back contact recombination velocity and ˆeBC is a normal vector

to ΣBC. For the edge of the space charge region, perfect collection is assumed (δn = 0).

Assuming that τ does not depend on δn, Equation 2.18 is a linear differential equation. The particle current (in units of s−1) across the edge of the space charge region Σp can

be expressed as:

I(´~x) = Z

Σp

De∇δn ˆep dσ, (2.19)

where ˆep is a normal vector to Σp. According to the reciprocity theorem derived in

References [14] and [13], the inhomogeneous differential equation 2.18 for δn(~x) can be substituted by a homogeneous differential equation for the collection function fc(~x):

De∆fc(~x) −

fc(~x)

τ = 0 (2.20)

Using as boundary conditions:

fc(~x) = 1 if ~x ∈ Σp −De∇fc(~x)ˆeBC = SBCfc(~x) if ~x ∈ ΣBC, it is obtained: a∗fc(´~x) = − Z Σp De∇δn ˆepdσ = I(´~x). (2.21)

Thus, the collection function fc(~x) corresponds to the normalized current response for

point like generation in the quasi neutral region, which is equivalent to the probability of an electron generated at position ´~x to be collected. At the edge of the space charge region, the collection probability is assumed to be one.

In a more general case of an extended generation profile, which can be described by the superposition of δ-functions, the collected current (in units of A) is obtained by integration over the generation volume V

I = e Z

V

g(~x)fc(~x)d~x. (2.22)

Thus, the electron current across the edge of the space charge region Σp, is expressed as a

convolution of fc(~x) and g(~x). In case of translation invariance parallel to the pn-junction,

Equation 2.22 simplifies to:

I = e Z

10 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

where x is the spatial coordinate perpendicular to the pn-junction and fc(x) and g(x) =

R R g(~x)dydz are the one dimensional expressions of the collection function and the gen-eration profile. In case of an infinite semiconductor (no back contact), a one dimensional solution for fc(x) is given by:

ϕ(x) = exp − x Le , (2.24) where Le = √

Deτ denotes the electron diffusion length. If the semiconductor is limited

by a back contact at position x = xBC with a recombination velocity of SBC, a solution

for fc(x) is given by:

fc(x) =
1
Lecosh
x−xBC
Le
− SBC
De sinh
x−xBC
Le
SBC
De sinh
_{x}
BC−xp
Le
+ _{L}1
ecosh
_{x}
BC−xp
Le
, (2.25)

where xp stands for the position of the edge of the space charge region.

### 2.3. IV characteristics

Diode equation

Based on the continuity equation, Shockley derived an equation for the dark current voltage characteristics of an ideal diode, which is given by [10, 15]:

jdiode(V ) = j0 exp eV kT − 1 with j0 = e pn0 Dh Lh + np0 De Le , (2.26)

where j0 is the saturation current density and V the applied voltage. np0 stands for the

equilibrium electron density on the p-side, pn0 for the equilibrium hole density on the

n-side, and Lh for the hole diffusion length. The simplifying assumptions necessary for

the derivation of this equation are abrupt depletion layers, the Boltzmann approximation for charge carrier densities, low injection conditions and no generation or recombination currents within the depletion layer [10].

The diode equation of a real diode can be expressed in the form:

jdiode(V ) = j0 exp eV AkT − 1 with j0 = j00exp − Ea AkT (2.27)

where A is the diode quality factor, Ea is the activation energy of the saturation current

density and j00 is a reference current density, which is weakly temperature dependent. A

detailed evaluation shows, that the values of A and Ea depend on the dominant

recombi-nation process within the solar cell [16, 17].

2.3 IV characteristics 11

the IV characteristics is given by:

jlight(V ) = j0 exp eV AkT − 1 − jphoto(V ) (2.28)

In the simplest case, the superposition principle holds meaning that the dark IV curve is only shifted by the value of a voltage independent photocurrent. But in real solar cells, the photocurrent can be voltage dependent and the diode current does not necessarily have to be the same in the dark as under illumination. In CIGSe solar cells, a crossing of the dark and illuminated IV curves is frequently observed, which is called ”cross over effect” [5, 18, 19]. In Figure 2.3, measured dark and illuminated IV curves of a CIGSe solar cell with an absorber layer with a Ga-content of [Ga]/([Ga]+[In]) =: Ga/III = 0.3 are shown. Besides the cross over effect (see Figure 2.3), there are other characteristic deviations from an IV curve according to Equation 2.28 observed for CIGSe solar cells: the so called roll over effect, i.e. a saturation of the current for V > VOC, [20] and the

(red) kink effect, which is treated in detail in the present work and is introduced in Section 3.3 (see Figure 3.6).

*j*

SC
*V*

OC
Figure 2.3: Dark and white light illuminated IV curves of a CIGSe solar cell with an absorber layer with a Ga-content of Ga/III = 0.3 measured at a temperature of 300 K. There is a crossing between the dark and the illuminated IV curves denoted as the ”cross over” effect.

Solar cell parameters

Characteristic solar cell parameters are the open circuit voltage (VOC), the short circuit

current density (jSC) and the fill factor (F F ), which is given by the ratio:

F F = Vmppjmpp VOCjSC

, (2.29)

where Vmpp and jmpp are the voltage and current density values at the point of maximum

12 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

cell is determined by:

η = F F jSCVOC Psun

, (2.30)

where Psun is the solar power density.

### 2.4. Recombination

The solar conversion efficiency of a solar cell is limited by the so called Shockley Queisser limit [21], which is determined by radiative recombination. The maximum efficiency of a solar cell with an absorber bandgap energy of 1.1 eV is calculated to be 30.1%. In CIGSe, also non radiative recombination via defect states in the bandgap takes place and record efficiencies are in the range of 20% [22]. In the following, an introduction is given into the basic equations describing non radiative recombination via a monoenergetic defect state in the bandgap according to the theory developed by Shockley, Read and Hall (denoted as SRH recombination) [23, 24].

Demarcation levels

In equilibrium, the occupation of all electronic states within a semiconductor is given by the Fermi distribution function given by Equation 2.13. The Fermi level corresponds to the energy level at which the occupation probability is 1/2. Under illumination in the steady state, the electron and hole Fermi levels Efn and Efp split up. They are given by:

EC− Efn = kT ln NC n EV− Efp = kT ln NV p (2.31)

The electron density corresponds to the sum of the density in equilibrium and the density of additionally generated electrons n = n0+ δn and the hole density correspondingly to

p = p0 + δp. The steady state quasi Fermi levels for electrons and holes describe the

occupation of those states which are still in effective thermal equilibrium with the bands [25]. In this case, the occupation is determined by thermal exchange with the respective band and not by recombination.

In the following, the case of a p-type semiconductor and electrons as its minority charge carriers are considered. A defect state is defined as a recombination center, if the proba-bility of re-emission of a trapped electron to the conduction band is smaller than that of emission to the valence band. Otherwise it is defined as an electron trap. The energetic level, at which the probabilities of re-emission to the conduction band and emission to the valence band (recombination) are equal, is denoted as demarcation level ¯En. It can be

2.4 Recombination 13

the hole Fermi level and the demarcation level: Efp< Et < ¯En. ¯En is given by [25]:

EC− ¯En= Efp+ kT ln

σem∗e

σhm∗h

(2.32)

where m∗_{e,h}are the effective masses of electrons and holes respectively. In the band diagram
shown in Figure 2.4, the region where defect states are efficient recombination centers is
shaded. Thus, if a defect level contributes significantly to non radiative recombination,
depends critically on its relative energy level within the bandgap, which in turn depends
on the local band bending, which is influenced by an external voltage and the charge
distribution within the device.

*E*

C
*E*

V
*E*

n
*E*

fn
*E*

fp
*E*

t
Figure 2.4: Band diagram of a p-type semiconductor. E¯n denotes the demarcation level. If

the energy level of a defect state Et is within the shaded area, the defect is an

effective recombination center. Otherwise a captured electron is more likely to be re-emitted to the conduction band and the defect state is denoted as a trap.

Occupation of recombination centers

The recombination rate of electrons via a monoenergetic recombination center in the bandgap is given by [12]:

Re= σevenNt,h (2.33)

where σeis the electron capture cross section of the defect state, veis the electron velocity

and Nt,h the density of those defect states occupied by a hole.

In the following, a homogeneously illuminated semiconductor with a monoenergetic accep-tor type defect state in open circuit conditions with a local recombination rate of electrons and holes equal to the local generation rate is assumed. Using that the thermal emission rate of electrons is proportional to the density of defect states occupied with an electron and assuming charge neutrality within the semiconductor, the occupation probability αt

of the defect state is given by [12]:

αt =

σeven + σhvhNVexp−Et_{kT}−EV

σeve n + NCexp−EC_{kT}−Et + σhvh(p + NVexp−Et_{kT}−EV)

(2.34)

where Et denotes the energetic level of the defect state, vh the hole velocity and σh the

14 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

Recombination rate

A p-type semiconductor with a single defect level of density Nt is considered in the

following. Electrons are minority charge carriers. The minimum lifetime of an electron τe0 is defined as the lifetime if all defects states are unoccupied. It is given by:

τe0 =

1 σevthNt

, (2.35)

where vth is the thermal velocity of the electron and σe denotes the capture cross section

of the recombination process. The principle processes involved in SRH recombination are: the capture of electrons and holes and the re-emission of electrons and holes. Based on the equation for the rates of these processes, the following fundamental equation for the net recombination rate for a monoenergetic defect level can be derived [26]:

R = np − n

2 i

γh(n + n∗) + γe(p + p∗)

(2.36)

In case of bulk recombination without tunneling, γe and γh correspond to the minimum

lifetimes of electrons and holes τe0 and τh0. The quantities n∗ and p∗ correspond to the

electron and hole densities if the Fermi energy is located at the defect energy level. For a defect level close to one of the bands, n∗ or p∗ is large and the recombination rate is small. On the other hand, if n∗ and p∗ are small, which is the case if the defect energy level is close to midgap, the recombination rate becomes large.

Using that np = n2_{i}exp eV_{kT}, Equation 2.36 can be transformed to:

R = n
2
i exp
eV
kT − 1
τh0[n + n∗] + τe0
h_{n}2
i
nexp
eV
kT + p
∗i
(2.37)

The maximum of recombination can be determined via the derivation of R with respect
to n:
dR
dn =
−n2
i exp
qV
kT − 1
h
τh0(n + n∗) + τe0
_{n}2
i
nexp
qV
kT + p
∗i2
τh− τe
n2
i
n2exp
qV
kT
(2.38)
and it is dR_{dn} = 0 for:
n
τe0
= p
τh0
(2.39)
Thus, if τe0 ≈ τh0 the position of maximum recombination is close to where p = n, which is

given within the space charge region of the pn-junction. The recombination rate gets lower the more asymmetric the electron and hole concentrations are, because the recombination process requires both, electrons and holes, to be present at the same position within the device.

2.4 Recombination 15

Interface recombination

Interfaces between different materials are critical with respect to recombination, because it is likely that the defect density is increased as compared to the bulk of the materials, because there are dangling bonds, unfavorable structural reconstruction, lattice mismatch and interdiffusion of atomic species from one material to the other. Interface recombina-tion processes may be described by the same equarecombina-tions as those of bulk recombinarecombina-tion, i.e. according to the SRH formalism.

For interface recombination without tunneling, γe and γh in Equation 2.36 are replaced

by S_{e,IF}−1 and S_{h,IF}−1 , where Se,IF and Se,IF stand for the recombination velocities of electrons

and holes at the interface, which are given by:

Se,IF= Nt,IFσeve and Sh,IF = Nt,IFσhvh, (2.40)

where Nt,IF is the interface defect density, σe,h denotes the capture cross sections for

electrons and holes and ve,h stands for the thermal velocities. The maximum interface

recombination velocity is determined by the thermal velocity of the charge carriers. For a given distribution of interface defects, the recombination probability of a photo generated electron at the interface depends on the availability of holes as recombination partners. Thus, one decisive quantity for interface recombination is the hole concentra-tion, which is given by the energetic difference between the valence band maximum and the hole Fermi level φh. The so called hole barrier φh is indicated by an arrow in the

electronic band diagram of the heterojunction region of a CuInSe2 (CISe) solar cell shown

in Figure 2.5.

**Φ****h**

CISe CdS ZnO

Figure 2.5: Electronic band diagram of the heterojunction region of a CISe solar cell. The arrow indicates the hole barrier at the absorber/buffer interface.

A large hole barrier at the interface, which is desirable in order to minimize interface recombination within the solar cell under illumination, is achieved by [27]:

• Asymmetric doping densities within the p- and n-type layers: Nd Na (n+p

junction).

• Positively charged interface defect states.

16 Chapter 2. Theory of charge carrier transport in heterojunction solar cells

• A spike in the conduction band at the interface.

• An enlarged bandgap energy at the absorber layer surface (interface to CdS) re-sulting from a locally lowered valence band maximum as possibly obtained by the formation of a surface ODC layer in CIGSe (see Section 3.2).

### 2.5. Thermionic emission across a potential barrier

*E*C
max
*E*cmin
*E*0
*xE0*0 *position x*

### (a)

### (b)

Figure 2.6: Detail sketch of the electronic band diagram including the conduction band min-imum and the electron Fermi level at a CIGSe/CdS heterojunction with a posi-tive conduction band offset (spike). In the classical approach within thermionic emission theory, electrons of sufficient energy can overcome the energetic barrier provided by the spike resulting in a thermionic emission current density jTE,e. In

thermionic field emission theory, quantum mechanical tunneling of electrons is also included (thermionic field emission current density jTFE,e).

Within thermionic emission (TE) theory, charge carrier transport across energetic barriers is described using classical concepts. A charge carrier is assumed to overcome an energetic barrier, if its energy is sufficient. Quantum mechanical tunneling is not considered. The basic equations were derived for metal-semiconductor contacts [10, 28], but can also be applied to semiconductor-heterojunctions exhibiting band offsets as energetic barriers. The IV characteristics of a metal-semiconductor contact according to thermionic emission theory is given by [28]: jTE = qNC,Vv¯e,h 4 exp −eφb kT exp eV kT − 1 , (2.41)

where NC and NV are the effective densities of states in the conduction and the valence

band, ¯ve and ¯vh are the average electron and hole velocities and φb is the barrier height.

φb corresponds to the energetic difference between the Fermi level (electron or hole) and

the corresponding band edge (conduction band minimum or valence band maximum). From this equation, the thermionic emission current of electrons across the CIGSe/CdS

2.6 Tunneling through a potential barrier 17

interface of a CIGSe solar cell with a conduction band spike ∆EC (see Figure 2.6) can be

deduced. It corresponds to the electron current from the CIGSe layer into the CdS layer minus the current from the CdS layer into the CIGSe layer [29] (V=0):

jTE,e = vth n(0+)exp −∆EC kT − n(0−) (2.42)

where n(0+_{) and n(0}−_{) are the electron densities on the CIGSe and the CdS side of the}

interface respectively. For simplification, the thermal velocities and the effective density of states in the conduction band are assumed to be equal in the CIGSe and the CdS layers. Thus, the electron current depends on the barrier height as well as on the electron densities on both sides of the junction. The electron density on the CdS side can be expressed as: n(0−) = n(0+)exp −∆EC kT exp −∆Efn kT (2.43) where ∆Efn is the offset in the electron Fermi level at the interface. Thus, jTE,e can be

expressed as: jTE,e = vthn(0+)exp −∆EC kT 1 − exp −∆Efn kT (2.44)

### 2.6. Tunneling through a potential barrier

In thermionic field emission theory, tunneling of charge carriers through an energetic barrier is also included in addition to thermionic emission [30]. The tunneling probability of a charge carrier depends on its energy and the barrier height and width. It is equal to one, if the energy of the charge carrier is larger than the energetic barrier (classical limit). In Figure 2.6, both processes - pure thermionic emission and tunneling - are indicated in an electronic band diagram of a CIGSe/CdS heterojunction. Using the WKB approximation as a boundary condition, the thermionic field emission current density jTFE,e of electrons

across an energetic barrier in the conduction band can be expressed as [30]:

jTFE,e = jTE,e(1 + δ) (2.45)

and δ is equal to:

δ = 1
kTexp
Emax
C
kT
Z Emax_{C}
Emin_{C}
exp −E0
kT
T (E0)dE0,
where Emax
C = E
0−

C is the maximum value of the conduction band minimum at the interface

(0-, CdS side). Emin

C is given by the maximum of the value of the conduction band

minimum at the interface on the absorber side (0+) and the value of the conduction band
minimum in the bulk of the CdS layer: max{E_{C}0+, ECdS

C } (in the case displayed in Figure

2.6 it is: Emin

C = ECCdS).

18 Chapter 2. Theory of charge carrier transport in heterojunction solar cells
[30]:
T (E0) = exp
−4π
h
RxE0
0 [2m
∗
e(EC(x) − E0)]
1
2dx
if E_{C}min ≤ E0 < ECmax
= 1 if E0 > ECmax, (2.46)

where m∗_{e} is the effective mass of electrons, h is the Planck constant and xE0is the position

where EC = E0within CdS (see Figure 2.6 (b)). Thus, the larger the width of the energetic

barrier, the smaller is the tunneling probability. This means that a higher doped CdS layer leads to an increased tunneling current across the conduction band spike.

## 3. Charge carrier transport in

## Cu(In,Ga)Se

_{2}

## solar cells

In this chapter, the fundamentals of Cu(In,Ga)Se2 (CIGSe) thfilm solar-cells are

in-troduced and a literature survey on relevant aspects concerning charge carrier transport is given. In Section 3.1, the device structure of CIGSe solar cells, the deposition pro-cesses for the individual layers, basic material properties of CIGSe and the electronic band diagram of a CIGSe solar cell are introduced. Since CIGSe solar cells consist of a complex multilayer stack with several interfaces between the individual layers, which play an important role in charge carrier transport, Section 3.2 focuses on relevant aspects concerning interfaces. An overview of experimental observations concerning generation dependent charge-carrier transport properties observed in IV and EBIC measurements on CIGSe solar cells and explanatory models is given in Section 3.3, which provides the framework of the investigations carried out for the present work.

### 3.1. Basics of Cu(In,Ga)Se

_{2}

### thin-film solar-cells

### 3.1.1. Solar cell configuration

In Figure 3.1, the stacking sequence of a CIGSe thin-film solar-cell is displayed schemat-ically (a) and in a scanning electron microscope (SEM) image of a polished solar cell cross-section. All solar cells investigated for the present study were fabricated at the Helmholtz-Zentrum Berlin and use soda lime glass as a substrate material. The solar cell itself consists of a multilayer stack out of a sputtered molybdenum back contact (≈ 1 µm), an evaporated CIGSe absorber layer (≈ 2 µm), a CdS buffer layer (≈ 50 nm) deposited in a chemical bath and a sputtered double layer of intrinsic ZnO (i-ZnO) and Al doped ZnO (Al:ZnO). On top of the ZnO window layer, a metallic contact grid out of Al and Ni is evaporated.

The CIGSe absorber layer is evaporated in a so called multistage coevaporation process [31] based on the three stage physical vapor deposition (PVD) process [32]. During the first stage, a layered precursor out of In, Ga and Se is deposited at a substrate temperature of 330◦C, where the evaporation of (In-Se) and that of (Ga-Se) are carried out separately in order to control the final Ga to In ratio of the CIGSe layer. During the second stage, Cu and Se are evaporated at a substrate temperature of 525◦C. The stoichiometric point of CIGSe is detected by means of laser light scattering [33, 34], and from then on, Cu

20 Chapter 3. Charge carrier transport in Cu(In,Ga)Se2 solar cells

and Se are evaporated until the layer has a Cu-content ([Cu]/([In]+[Ga]) =: Cu/III) of approximately 1.15 (Stage 2a, where t2a = 0.15 t2). The fact that the film becomes

Cu-rich during the deposition process has an important influence on crystal growth most probably due to the segregation of a Cu-Se secondary phase at the surface of the CIGSe grains [35–37]. During stage three, In, Ga and Se are evaporated simultaneously and the process is terminated once the composition of the CIGSe layer becomes Cu-poor in the range of Cu/III= 0.7 - 0.9. In Figure 3.2, the multistage process used for CIGSe layer deposition of the investigated solar cells is displayed schematically.

The pn-junction of the solar cell forms between the p-type CIGSe absorber layer and the n-type CdS and ZnO layers. CdS is the standard material used as buffer layer in CIGSe thin-film solar-cells. It has a bandgap energy of 2.4 eV and thus absorbs part of the solar spectrum. With CdS as a buffer layer, the solar cells with the best conversion efficiencies are fabricated [22, 38], but since it is toxic and due to its unfavorably small bandgap energy, considerable effort is made to replace CdS by alternative materials like for example In2S3, ZnS and Zn(O,S) [39–41]. The ZnO layer serves as a transparent front

contact - a so called window layer. It is transparent for visible light due to its large band gap energy (3.3 eV) and has a good conductivity due to its high doping density. General review papers about CIGSe solar cells are given by References [38] and [42].

**CIGSe**

**ZnO**

**CdS**

**Mo**

**(a)**

**(b)**

**Ni/Al grid**

**1 µm**

Figure 3.1: (a) Schematic of the stacking sequence of a CIGSe thin-film solar-cell (b) SEM image of a polished cross section of a CIGSe thin-film solar-cell.

### 3.1.2. Material properties of Cu(In,Ga)Se

2CuInx−1GaxSe2 (CIGSe) is a direct semiconductor with a bandgap energy which depends

on the Ga-content x = [Ga]/([Ga]+[In]) =: Ga/III of the solid solution out of CuInSe2

(CISe) and CuGaSe2 (CGSe) and varies in between 1.04 eV (CISe) and 1.68 eV (CGSe).

3.1 Basics of Cu(In,Ga)Se2 thin-film solar-cells 21 time flux (a.u.) Ga Ga In In In Se t1 t2 t3 stoichiometric point t2a Cu Ga

Figure 3.2: Schematic of the multistage PVD process for CIGSe absorber deposition.

Eg(x) = (1 − x)EgCISe + xE CGSe

g − bx(1 − x) (3.1)

where b denotes the optical bowing coefficient, for which values ranging from -0.07 to 0.24 were determined experimentally [43]. First principle calculations show, that the increase in bandgap energy upon the addition of Ga is mainly due to an upward shift of the conduction band [44].

The crystal structure of CIGSe is the tetragonal chalcopyrite lattice, which can be deduced from the cubic sphalerite (zincblende) structure by doubling the unit cell. Unlike in semiconductors like Si or GaAs, where foreign atoms are used for doping the materials, the p-type doping of CIGSe results from intrinsic defects. There are 12 intrinsic point defects in CuInSe2 (CISe): three vacancies VSe, VIn and VCu, three interstitials Sei, Ini

and Cui and six antisite defects SeIn, SeCu, InSe, InCu, CuSe and CuIn.

CIGSe layers used as absorber layers in high efficiency solar cells exhibit non stoichiometric compositions with Cu/III= 0.7-0.9. An explanation, why such a defective material can still have appropriate electronic properties to be used as absorber layer in a solar cell is given by calculations based on density functional theory (DFT) [45]. It was shown, that the formation energies of Cu-vacancies VCu and the neutral defect complex (2V−Cu+ In

2+ Cu)

is particularly small and in some cases even negative. VCu forms a shallow acceptor,

which is thought to be responsible for the intrinsic p-type doping in CIGSe [45]. It
is further suggested that due to the formation of the (2V−_{Cu} + In2+_{Cu}) complex, CIGSe is
highly compensated with an effective doping density in the range of 1014_{to 10}16_{cm}−3_{. The}

pairing induces a very shallow level close to the conduction band, which is consequently
not acting as an effective recombination center. Thus, the formation of the defect complex
(2V−_{Cu}+In2+_{Cu}) may explain the electrically benign character of a large defect density present
in non stoichiometric CIGSe.

22 Chapter 3. Charge carrier transport in Cu(In,Ga)Se2 solar cells

### 3.1.3. Electronic band diagram of the solar cell

In Figure 3.3, an exemplary electronic band diagram of a CuInSe2 (CISe) thin-film

solar-cell is shown. The solar solar-cell consists of 4 layers: a CuInSe2 absorber layer (Eg = 1 eV),

a CdS layer, an i-ZnO and an Al:ZnO layer. The pn-junction forms between the p-type CISe layer and the n-type CdS and ZnO layers. Since the CISe absorber doping density is assumed to be lower than that of the n-type layers, most of the built in voltage drops across the CISe layer (see Equation 2.4). The absolute value of the conduction band offsets at the CISe/CdS and the CdS/ZnO interfaces are assumed to be 100 meV.

There are still open questions about the electronic band diagram of CIGSe solar cells, which will be addressed in more detail in the following:

• What are the band offsets at the heterointerfaces?

• What are the effective doping densities of the individual layers and how do they change upon illumination or the application of a voltage bias?

• Is the absorber doping density spatially homogeneous?

• Are there interface defects and what role do they play? Is there Fermi level pinning due to interface defects?

• What is the configuration of the CIGSe surface? Is there structural reconstruction leading to the formation of a secondary phase with a larger bandgap energy?

ZnO CdS CISe

Figure 3.3: Electronic band diagram of a CISe thin-film solar-cell.

### 3.2. Interfaces in Cu(In,Ga)Se

_{2}

### thin-film solar-cells

Surfaces of individual semiconductor layers and interfaces between different semiconductor layers are regions where the order of the crystal atoms is perturbed severely. An increased density of electronic defect states in the bandgap as compared to the bulk of the materials is likely to occur. Furthermore, interdiffusion of atoms between the different materials is possible, which can lead to defect states and the formation of additional phases. Another

3.2 Interfaces in Cu(In,Ga)Se2 thin-film solar-cells 23

critical point is the band alignment between materials of different electron affinities and bandgap energies. Since these issues are all relevant for charge carrier transport and device performance, they have been investigated and treated intensively in literature.

Elemental intermixing at the Cu(In,Ga)Se2/CdS interface

It has been found experimentally, that there is diffusion and intermixing of atomic species at the CIGSe/CdS interface and that the picture of an abrupt junction is not realistic. There are several publications reporting of the diffusion of Cd into the absorber layer or into its surface region [46–50]. The presence of Cd in the near-surface region is accompa-nied by a depletion of Cu. It is concluded that Cd occupies Cu sites and in this way acts as a donor defect state [51] causing inversion of the surface region and a buried pn-junction within the CIGSe layer [46–49], which was also detected by means of Kelvin Probe Force Microscopy (KPFM) measurements [52]. However, a buried pn-junction was also found in devices without CdS and might be caused by an n-type ordered defect compound (ODC) present at the surface of the CIGSe layer [53]. Other experimental results indicate an intermixing including the elements S, Se and In in the near-surface region leading to the formation of Cd(S,Se), CdIn(S,Se) and CuIn(S,Se)2 layers [54].

The Cu(In,Ga)Se2 surface

The configuration of the surface of the CIGSe layer as an individual layer and that of the region of the CIGSe layer close to the absorber/buffer interface in a completed solar cell are still not understood properly and discussed controversially in literature.

Calculations using the local density approximation (LDA) of density functional theory (DFT) show that the electrically neutral defect pair (2VCu-InCu) exhibits a low formation

energy [45, 55]. An attractive interaction between defect complexes may lead to the formation of ordered defect arrays, which form compounds like CuIn5Se8 and CuIn3Se5

(ordered defects compounds, ODCs) [45, 55]. The bandgap energies of these compounds are larger than that of CuInSe2: Eg,CuIn5Se8 = 1.34 eV and Eg,CuIn3Se5 = 1.26 eV [45].

Several photoelectron spectroscopy studies provide experimental evidence for the existence of an ODC layer with a larger bandgap energy at the surface of Cu poor CISe [53, 56, 57] as well as CuGaSe2 [58] and other Cu(In,Ga)(Se,S)2 compounds [59]. Results concerning

band offsets at the ODC/CISe interface are inconsistent. Different studies by Schmid et al. determine the conduction band offset to be ∆EC = 0.29 eV [53] and 0.02 eV [56], while

first principle calculations lead to a value of 0.17 eV [45]. As possible mechanisms for an increased Cu-depletion at the CIGSe surface, the formation of Cu-vacancies due to an upward shift of the Fermi level upon junction formation and field induced Cu-migration were suggested [60–63].

While the presence of a Cu-depleted surface is a frequent observation, there are ambiguous results concerning the existence of an ODC layer with a larger bandgap energy than the bulk material. There are studies indicating that Cu-depletion only occurs within the top atomic layers of a CIGSe surface and that there are no secondary phases formed [49, 64, 65].

24 Chapter 3. Charge carrier transport in Cu(In,Ga)Se2 solar cells

that in CIGSe solar cells with Cu-poor absorber layers of different bandgap energies, bulk recombination dominates, while in solar cells with Cu-rich CIGSe layers interface recombination prevails [66]. This behavior was ascribed to the presence of an ODC layer at the CIGSe/CdS interface with a lowered valence band maximum as compared to the CIGSe layer in solar cells with a Cu-poor absorber layer. The local hole barrier is in this case increased, which may lead to reduced recombination via interface defects [66, 67]. Numerical simulations confirm the increase of the open circuit voltage in the presence of an ODC phase at the absorber layer surface (interface to CdS) [68].

Interface states and Fermi level pinning at the Cu(In,Ga)Se2/CdS interface

Charged interface defects might play an important role concerning charge and potential distributions in a CIGSe solar cell. If the defect concentration of a donor type interface defect is high enough to compensate the negative charge within the p-type layer, the elec-tron Fermi level is pinned at the interface. This means that the local energy difference between the electron Fermi level and the conduction band minimum does not change if a voltage bias is applied. In this case, the interface defect instead of the n-type layers contributes the positive charge of the pn-junction, and changes in potential drop across the pn-junction of the solar cell due to an applied external bias are compensated by a change in the occupation of the defect state.

In Figure 3.4 (a), electronic band diagrams of the heterojunction region of a CISe solar cell with a monoenergetic interface donor state with a density of Nt,IF = 1013cm−2 are

shown for defect energy levels of Et,IF = EC,CISe - 0.1 eV and EC,CISe -0.2 eV. The Fermi

level is pinned close to the defect energy level. A shallower defect leads to a higher degree of inversion/ smaller hole density at the interface. Numerical simulations show that an increased degree of inversion due to Fermi level pinning by donor type interface states can lead to an increased open circuit voltage of the solar cell [68].

Based on a detailed evaluation of admittance spectra of CIGSe solar cells - especially the interpretation of a characteristic admittance step called N1 admittance step - Herberholz et al. [69] introduced a model of an energetically continuous distribution of donor type interface defects present at the CIGSe/CdS interface. The defect density is assumed to be high enough to cause Fermi level pinning at the interface. In Figure 3.4 (b), this situation is displayed for two different defect densities. For a higher defect density, the Fermi level is pinned closer to the conduction band minimum, because the charge accumulated in the defect states with an energy level above the Fermi level is sufficient to compensate the charge in the CIGSe layer. Within this model, the activation energy of the N1 admit-tance step, which can be determined experimentally, corresponds to the energy difference between the electron Fermi level and the conduction band minimum at the CIGSe/CdS interface. Alternative interpretations ascribe the N1 admittance step to a bulk acceptor level [70], a barrier at the Mo/CIGSe back contact [20] or a mobility freeze out at low temperatures [71].

The presence of interface defects might also be one of the reasons, why the open circuit voltage of CIGSe solar cells does not increase as expected for an increase in bandgap energy of the absorber layer upon the addition of Ga [72, 73]. If there is a high den-sity of interface defects at the same energetic difference from the valence band maximum independent of the Ga-content such that the Fermi level is pinned, the open circuit

volt-3.2 Interfaces in Cu(In,Ga)Se2 thin-film solar-cells 25

### (a)

### (b)

IF 1 IF 1

Figure 3.4: (a) Detail sketch of the electronic band diagrams of the heterojunction region of a CISe solar cell for monoenergetic donor type interface defects at the CISe/CdS interface (denoted as IF1) for two different energy levels (Nt,IF = 1013cm−2). (b)

Detail sketch of the electronic band diagrams of the heterojunction region of a CISe solar cell for an energetically continuous distribution of donor type interface defects (uniform distribution) at the CISe/CdS interface (IF1) for two different integrated defect densities Nt,IF = 5 × 1013cm−2 and 5 × 1012cm−2.

age does not depend on the absorber bandgap energy [73]. In this case, the dominant recombination mechanism changes from bulk recombination for small absorber bandgap energies to interface recombination for wide bandgap absorber layers.

Band alignment at the Cu(In,Ga)Se2/CdS interface

Band alignment at the CIGSe/CdS interface in thin-film solar-cells is still not understood properly: Band offsets are not quantified and the way in which they influence charge carrier transport is still an open question. In literature, contradictory results concerning the conduction band offset at the CISe/CdS and the CIGSe/CdS interfaces are presented. In the following, a conduction band offset is denoted as a spike, if the electron affinity of CIGSe is larger than that of CdS and as a cliff if the electron affinity of CIGSe is smaller than that of CdS. These two scenarios are visualized in Figure 3.5.

While some publications suggest a rather large spike of 0.3 eV [53] (between a surface ODC layer and CdS), 0.5 eV [74] or even 0.7 eV, [75] at the CuInSe2/CdS interface,

others assume a small spike or flatband alignment [5, 57], or even a small cliff of -0.08 eV [76]. First principle calculations determined a spike of 0.31 eV between CuInSe2 and

CdS [77]. The addition of Ga into the absorber layer increases the bandgap energy of the material and calculations and experimental data indicate that the addition of Ga leads to an upward shift of the conduction band changing the band alignment from a spike to a cliff configuration [43, 72, 78].

A spike in the conduction band serves as an energetic barrier for electrons from the ab-sorber layer. It depends on the barrier height and width, temperature and the electron concentration at the interface if the electron current is reduced by the conduction band offset (see also Section 2.5 and 2.6). Niemegeers et al. [29] showed that for a moderate

26 Chapter 3. Charge carrier transport in Cu(In,Ga)Se2 solar cells

Figure 3.5: Detail sketch of the electronic band diagrams of the interface region of CISe so-lar cells assuming a spike and a cliff at the CISe/CdS interface (300 meV). No conduction band offset at the CdS/ZnO interface is assumed.

spike, electron transport across the heterojunction is not affected severely. If there are midgap interface states, a spike can even have a positive effect by increasing the local hole barrier (see Section 2.4). This means that the local hole density is reduced and there are less recombination partners for electrons from the absorber layer, which reduces interface recombination. A conduction band cliff on the other hand leads to a reduced hole barrier and might in this way increase interface recombination [27].

### 3.3. Generation dependent charge-carrier transport

### properties

In this section, a detailed overview of experimental observations reported in literature and proposed models concerning the occurrence of generation dependent charge-carrier transport properties of CIGSe solar cells is given.

### 3.3.1. Experimental observations

Under certain experimental conditions, a characteristic phenomenon observed in IV mea-surements on CIGSe solar cells is the so called kink effect, i.e. a severe reduction of the measured photocurrent under forward bias (V < VOC) resulting in a low fill factor [2–

4, 6, 8, 79–85]. The effect is called red kink if it occurs under illumination containing only the red part of the solar spectrum (no absorption in the CdS layer). In Figure 3.6, typical IV curves measured at a temperature of 100 K using red and white light illumination of a CuInSe2 solar cell are shown. While the fill factor of the white light illuminated IV

curve is 84.8%, it is only 55.3% for red light illumination. Thus, charge-carrier transport properties are generation dependent.